investigating and preventing premature deterioration ?· investigating and preventing premature...
Post on 15-Aug-2018
Embed Size (px)
Investigating and Preventing Premature Deterioration of Colored Concrete PavementWhat Was the Need?The use of colored concrete in pavement projects has gained popularity in Minnesota in recent years. Colored concrete may improve safety when used to delineate criti-cal road features and so provide guidance to pedestrians and drivers. It is also used simply to look appealing.
Many colored concrete pavement projects in Minnesota have displayed microcracking near contraction joints. While this type of distress also happens in regular con-crete pavements, it appears to be accelerated in colored concrete pavements, with deterioration observed within five years of construction in some instances.
For colored concrete to be practical for continued usage in Minnesota pavements, agencies need to have confidence in its durability. However, there was little published research on the performance of colored concrete that might identify the cause of or remedy for premature deterioration.
What Was Our Goal?This project sought to determine the causes of premature distress in Minnesota colored concrete pavement projects and identify suitable repair and rehabilitation techniques for projects that have suffered this distress.
What Did We Do?Researchers first identified 45 projects in Minnesota that included colored concrete pavement, sidewalks or medians, and collected data about each project including its construction date and any distresses observed. They visited several of these projects as well as three current construction sites where they could observe construction practices for colored concrete.
Then 17 core samples were collected from four projects that had experienced signifi-cant early distress. Researchers conducted petrographic analysis in accordance with ASTM standard C856 on 11 of the core samples to determine a variety of characteristics for each, including an estimate of the water-to-cementitious materials ratio. The purpose of this analysis was to determine if early deterioration was caused by poor workmanship or the components within colored concrete.
Based on observations and knowledge from pavement experts, researchers recom-mended construction methods, mix designs, and repair and rehabilitation techniques for colored concrete.
What Did We Learn?Researchers did not identify a conclusive reason for premature distress in colored concrete. High porosity caused by high water-to-cementitious materials ratio mixes was commonly found and thought to likely have increased the tendency toward reduced freeze-thaw durability of the mixes. The presence of magnesium from deicers in con-crete pores may also be a cause, but the sample size was too small to confirm it as a definitive cause.
2014-26TS Published October 2014
Technical Liaison:Dallas Larson, City of Centerville
Project Coordinator:Bruce Holdhusen, MnDOT
Principal Investigator:Tom Burnham, MnDOT
Many samples had air voids filled with ettringite crystals (highlighted in red), which
reduce freeze-thaw resistance.
LRRB PROJECT COST:$37,435
might help prevent the
premature deterioration of
colored concrete pavements,
including controlling the
material ratio of the mix
and properly consolidating
and curing the pavement.
& LIBRARYO F F I C E O F T R A N S P O R T A T I O N
S Y S T E M M A N A G E M E N T
Researchers made several recommendations for improving the mix and construction of colored concrete. These include a maximum water-to-cementitious materials ratio of 0.43 for colored concrete placed in climates like Minnesotas. Higher ratios correspond with higher porosity, which allows more moisture and deicing chemicals into the con-crete and reduces its freeze-thaw resistance. Core samples from only one of the colored concrete sites tested had average water-to-cementitious materials values below 0.45. Researchers also recommended specifying a total air content in the mix of 7.0 percent before consolidation to create a well-distributed air void system. Laboratory testing suggested that the pigments used to color concrete have little impact on its freeze-thaw durability.
Several core samples showed evidence of chemical attack of the cement paste and fine aggregates, and alkali-silica reaction, which can cause cracking or spalling. Finding ASR was surprising since these mixes used the same aggregates as standard concrete, which does not typically develop ASR in Minnesota pavements.
Since colored concrete is typically used in relatively small areas, it is usually placed and formed without mechanical equipment. While construction techniques were not found to be the primary cause of concrete distress, researchers did make some construction recommendations. These include using mechanical vibration when possible to level and consolidate the concrete, making provisions for the difference in thermal expansion between different colored concrete mixes and devising improved methods for curing.
Standard repair and rehabilitation techniques should work for colored concrete pave-ment. However, when damage is expansive or rapidly developing, full slab replacement is often the only viable option.
Whats Next?The ready-mix colored concrete industry has recognized the seriousness of poor dura-bility and is working to educate producers and placers about the need for proper mix design, placement techniques and curing procedures. Agencies considering the use of colored concrete should be careful to consider whether it can be produced and placed properly. Concrete stains, pavers or colored high-friction surface treatments may be ap-propriate alternatives to consider.
These research results were presented at the TERRA Pavement Conference, and a webi-nar is planned to help publicize this work.
Further research may be warranted to determine whether following best practices pro-vides the expected improvement in colored concrete durability. It may also be worth-while to investigate the cause of chemical attack that was discovered during this project.
Produced by CTC & Associates for: Minnesota Department
of Transportation Research Services & Library
MS 330, First Floor 395 John Ireland Blvd.
St. Paul, MN 55155-1899651-366-3780
www.mndot.gov/researchThis Technical Summary pertains to the LRRB-produced Report 2014-26, Investigation and Assessment of Colored Concrete Pavement, published August 2014. The full report can be accessed at http://www.lrrb.org/PDF/201426.pdf.
Many Minnesota colored concrete projects have experienced premature distress, including this intersection in Centerville. Joint deterioration began to appear in 2011, just three years after the intersection was constructed.
Many variables can impact the end result of a colored concrete project that are not easy to control. I dont think I could ever justify doing another colored concrete project.
Dallas Larson,City Administrator, City of Centerville
We dont want to eliminate colored concrete technology if it can be done properly.
Tom Burnham,Senior Road Research Engineer, MnDOT Office of Materials and Road Researchwww.terraroadalliance.org/events/conference/2014/documents/6_Burnham.pdfhttp://www.mndot.gov/researchhttp://www.lrrb.org/PDF/201426.pdf